Preparation and characterization of chitosanâ€“caboxymethyl ... Cu (II) and Cr (IV)...
Embed Size (px)
Transcript of Preparation and characterization of chitosanâ€“caboxymethyl ... Cu (II) and Cr (IV)...
Instructions for use
Title Preparation and characterization of chitosancaboxymethyl--cyclodextrin entrapped nanozero-valent iron compositefor Cu (II) and Cr (IV) removal from wastewater
Author(s) Sikder, Md. Tajuddin; Mihara, Yoshihiro; Islam, Md. Shariful; Saito, Takeshi; Tanaka, Shunitz; Kurasaki, Masaaki
Citation Chemical Engineering Journal, 236: 378-387
Issue Date 2014-01-15
Doc URL http://hdl.handle.net/2115/53586
Type article (author version)
Additional Information There are other files related to this item in HUSCAP. Check the above URL.
File Information Revised Manuscript.pdf
Hokkaido University Collection of Scholarly and Academic Papers : HUSCAP
Preparation and characterization of chitosan-caboxymethyl--cyclodextrin entrapped nano
zero-valent iron composite for Cu (II) and Cr (IV) removal from wastewater
Md. Tajuddin Sikdera, b, Yoshihiro Miharac, Md. Shariful Islama, Takeshi Saitod, Shunitz Tanakaa,
e, Masaaki Kurasakia, e, *
aDivision of Environmental Science Development, Graduate School of Environmental Science,
Hokkaido University, 060-0810 Sapporo, Japan.
bDepartment of Environmental Science, Stamford University Bangladesh, Dhaka-1209,
cDivision of Environmental Materials Science, Graduate School of Environmental Science,
Hokkaido University, 060-0810 Sapporo, Japan.
dGroup of Environmental Adaptation Science, Faculty of Environmental Earth Science,
Hokkaido University, 060-0812 Sapporo, Japan.
eLaboratory of Environmental Health Sciences, Faculty of Health Sciences, Hokkaido University,
060-0812 Sapporo, Japan.
*Corresponding author: Dr. Masaaki Kurasaki, Group of Environmental Adaptation Science,
Faculty of Environmental Earth Science, Hokkaido University. Kita 10, Nishi 5, Kita-ku,
Sapporo 060-0810, Japan.
Tel: +81-11-706-2243; fax: +81-11-706-4864
The entrapment of Fe0 nanoparticles within a chitosan-carboxymethyl -cyclodextrin complex, a
nontoxic and biodegradable stabilizer, yields chitosan-Fe0 nanoparticle-carboxymethyl -
cyclodextrin beads that are 2.5 mm in diameter and contain 50% iron by weight. The complete
disappearance of Cr (VI) and Cu (II) may involve both physical adsorption and reduction of Cr
(VI) to Cr (III) and Cu (II) to Cu (0) while oxidizing Fe0 to Fe (III). The rate of reduction can be
expressed by pseudo-second-order reaction kinetics. The rate constants increased with increasing
iron loading and initial concentration at pH 6, while the adsorption of Cr (VI) and Cu (II) was
found to be endothermic and exothermic, respectively. The apparent activation energies for Cr
(VI) and Cu (II) were found to be 71.99 and 18.38 kJ mol1, respectively. X-ray photoelectron
spectroscopy confirmed the reduction process. The equilibrium data could be well described by
both Langmuir and Temkin isotherms for describing monolayer adsorption and chemisorption
processes, respectively. Both film diffusion and intraparticle diffusion were found to be the rate-
limiting steps from the analysis of an intraparticle diffusion model. Thus, the synthesized
chitosan-Fe0-nanoparticle-carboxymethyl -cyclodextrin beads can be a potential material for in
situ remediation of contaminated surface and ground water.
Keywords: Chitosan, zero-valent iron, remediation, cyclodextrin polymer, heavy metals, water
Toxic heavy-metal pollution is of significant environmental and occupational concern because of
the tendency of heavy metals to enter the food chain. Among metals of concern, chromate (Cr
(VI)) is the 16th most toxic and carcinogenic material released into the environment through
numerous industrial operations . Cu (II) is toxic at elevated concentrations, and is persistent
and bioaccumulative in the environment. Cr (VI) concentrations range from 0.5 to 270 mg L-1 in
industrial wastewater [2, 3], though the US Environmental Protection Agency (EPA) permissible
limit of Cr (VI) is only 0.1 mg L-1. The acceptable limits for Cu (II) set by the EPA and WHO
(2011) are 1.2 and 2 mg L-1, respectively [4-6]. Numerous studies have investigated adsorption
and redox processes as removal mechanisms of Cu (II) and Cr (VI) from water using of a variety
of materials including natural adsorbents, waste materials, microorganisms and macromolecules
[3, 7-14]. Recently, adsorption using nano zero-valent iron (NZVI), chitosan (CS), and
carboxymethyl -cyclodextrin (CM-CD) has attracted increased attention for use in
environmental remediation of heavy-metal ions.
Zero-valent iron powders (Fe0) have been extensively used for in situ remediation of water
polluted with As , chlorinated hydrocarbons , nitrate , Cr (VI), and Pb (II) .
Special attention has recently given to insoluble form of NZVI because of its large surface area
and tremendous reducing capacity for heavy metals . In addition, the oxidation of NZVI by
water and oxygen produces ferrous iron to give magnetite, depending upon redox conditions and
pH . This process, rendering the iron magnetic, facilitates the rapid separation of adsorbents
CS is an important natural polymer, obtained by the deacetylation of chitin, in which the
amino group has a pKa value from 6.2 to 7.0, positively charged and soluble in acidic-to-neutral
solution, and has found extensive application in the green synthesis of nanoscale materials
because of its excellent biocompatibility, biodegradability, and lack of toxicity. Recently,
adsorption of metal ions to CS has been extensively studied because CS exerts bioadhesive
properties to form stable nanoparticles with different metals in solution [19, 20]. Because the
amino groups of CS have the ability to form chelation complexes with various heavy-metal ions,
CS has been used as a material for environmental remediation .
-CD is a cyclic oligosaccharide containing a hydrophobic, a polar cavity with hydroxyl
groups present on the inside and outside of the cavity. There is evidence that both organic and
inorganic compounds can complex with -CD through its cavity and hydroxyl groups [7, 22].
Recently, -CD has been immobilized or grafted with supportive materials, and active functional
groups have been introduced to enhance its adsorption capacity for metal ions, e.g., CM-CD.
The coupling of CM-CD with functionalized CS followed by the entrapment of NZVI is
expected in this study to facilitate the removal of metals from wastewater.
In water treatment systems, direct application of NZVI may cause iron pollution because of its
tiny particle size. In addition, NZVI exhibits high agglomeration, high mobility, lack of stability,
and low reducing specificity in water, and thus must be used with surface stabilizers such as CS,
alginate, activated carbon, and others porous structures . If these supporting materials also
have high affinity for metal ions, the combination with NZVI accelerates the overall remediation
process. The use of CS as stabilizer can facilitate detoxification of metal ions in solution and act
as effective electron donor. In addition, the sorption mechanism along with the degree of
detoxification of heavy metal ions is also known [12, 24-26]. Some papers have reported only
CS bearing NZVI beads for Cr (VI) and Cu (II) removal, but have not specially studied the
thermodynamics, kinetics and isotherms extensively; and the removal mechanism was not
elucidated clearly for metal ions [12, 21, 24-30]. In this study, NZVI was entrapped in a highly-
functioning, porous polymer CS already cross-linked with CM-CD to yield CS-NZVI-CM-CD
beads. The adsorption behavior of CS-NZVI-CM-CD beads were fabricated and their
adsorption behavior was characterized using Cu (II) and Cr (VI) ions in solution. The adsorption
mechanism, characteristics, thermodynamics, influence of different factors, kinetics, and
isotherms of CS-NZVI-CM-CD beads were also evaluated.
2. Materials and methods
Deacetylated CS flakes (75%), called 2-amino-2-deoxy-(1-4)--D-glucopyranan or poly-(1,4)--
D-glucopyranose amine, derived from shrimp shells and CM-CD sodium salt were purchased
from Sigma-Aldrich (St. Louis, MA, USA). NZVI electrolytic powder finer than 100 mesh, 98%
purity, was purchased from Kanto Chemical (Tokyo, Japan). Condensation reagent for the
synthesis of 1,3-bis(2,2-diethyl-1,3-dioxolan-4-yl-methyl) carbodiimide was purchased from
Tokyo Chemical Industry (Tokyo, Japan). All other chemicals were of analytical grade. Milli-Q
water (Millipore-Gradient A10, Milli-Q Gradient ZMQG) was used in the experiments.
2.2 Preparation of CS-CM-CD gel
CS-NZVI-CM-CD beads were prepared using the commercially available CS flakes, CM-CD
sodium salt, and NZVI. First, 1,000 ppm CM--CD sodium salt in 500 mL of water was
equilibrated with 2% (v/v) acetic acid. The mixture was stirred for 8 h at room temperature. Then,
CS flakes without depolymerization (4.0 g) were added in small portions to 200 mL of the
mixture at 333 K, which was stirred for 6 h followed by cooling to 293 K to obtain CS-CM-CD